# RECENT FINITE ELEMENT STUDIES IN PLASTICITY esag. 18(~979)411-442 @north-hollandpublishingcompany...

date post

23-May-2018Category

## Documents

view

214download

1

Embed Size (px)

### Transcript of RECENT FINITE ELEMENT STUDIES IN PLASTICITY esag. 18(~979)411-442 @north-hollandpublishingcompany...

COMPUTERMETHODSINAPPLIEDMECHANICSANDENGINEERING17~18(~979)411-442 @NORTH-HOLLANDPUBLISHINGCOMPANY

RECENT FINITE ELEMENT STUDIES IN PLASTICITY AND FRACTURE MECHANICS

James R. RICE Brown University, Providence, R.I., U.S.A.

Robert M. McMEEKING University of Illinois, Urbana, Ill., U.S.A.

David M. PARKS Yale ~?~iversity, New Haven, Corm., U.S.A.

and

E. Paul SORENSEN General Motors Research Laboratories, Warnen, Mich., USA.

The paper reviews recent work on fundamentals of elastic-plastic finite-element analysis and its applications to the mechanics of crack opening and growth in ductile solids. The presentation begins with a precise formu~tion of in- cremental equilibrium equations and their finite-element forms in a marines valid for deformations of arbitrary mag- nitude. Special features of computational procedures are outlined for accuracy in view of the near-incompressibility of elastic-plastic response. Applications to crack mechanics include the analysis of large plastic deformations at a progressively opening crack tip, the determination of J integral values and of limitations to I characterizations of the intensity of the crack tip field, and the determination of crack tip fields in stable crack growth.

Introduction

Our paper begins with fundamentals of elastic-plastic finite-element analysis for deformations of arbitrary magnitude. Here there is a close association with the pioneering studies of Professor W. Prager on the foundations of plasticity theory and the mechanics of continua, and of Professor J.H. Argyris on the finite-element analysis of elastic-plastic and other non-linear prob- lems in structural mechanics; the paper is dedicated to them in honor of their respective 75th and 65th anniversaries. After reviewing the fundamentals we discuss recent computational solutions for crack tip defo~ations in elastic-plastic fracture mechanics. As we use the term for the present discussion, plasticity will refer to strain-rate insensitive inelastic response.

1. Incremental elastic-plastic formulation for deformations of arbitrary magnitude

The finite-element analysis of elastic-plastic continua was begun by Argyris I 11, Pope [2] , Swedlow et al. [31, and Marcaf and King [4] within the geometrically linear (or small strain) approximation. Oden [S] reviews finite-element formulations in the non-linear elasticity context for arbitrary strains. The first elastic-plastic formulation appropriate to deformations of arbitrary magnitude was given by Hibbitt, Marcal and Rice [61, and related fo~ulations, based likewise on

412 J. R Rice et al. fRecent finite element studies in plasticit) and fracture mechanics

suitably spin-invariant generalizations of the Prandtl-Reuss equations and accompanied by numeri-

cal examples, were given by Needleman [ 7, 81 and Osias and Swedlow 191. Later, McMeeking and Rice [ IO] showed the relation of these formulations to Hills [ 1 1 ] variational principle for incremental deformations, demonstrated the relation of the constitutive and initial stress stiffness matrices to the adopted measures of stress and strain, and discussed various proposed approaches for large-strain analysis in light of the rigorous formulation. We follow the presentation by

McMeeking and Rice in this review. In its reference configuration the body considered occupies the region V with surface So, and

position vectors of its particles are denoted by X. In its current configuration the same quantities

are given by V, S and x. Then, following Hill [ 111, the conditions for continuing equilibrium in incremental deformations are given by a rate form of the virtual work equation

for arbitrary 6x, where 6x is understood to vanish on the portions of So where x is prescribed. Here the notation is dyadic; t is the nominal stress (nits transpose is sometimes referred to as the first Piola-Kirchhoff stress); b is the body force per unit volume of reference state;f is the surface

force per unit area of reference state v= na . t at a surface element having normal no in the reference state). The superposed dpts denote time rates and it is well to recognize that in typical

problems the nominal force rates f may not be fully prescribed on So -- e.g., a rate of fluid pressure may be prescribed. In such cases f can be split additively (see [ 61) into a prescribed part and another part of geometric origin which is linear in ai/dX. The latter joins ), also a function of &/ax, on the left side of (I) as part of the unknown rate field x to be determined and contributes an initial load term to the overall stiffness.

There are many approaches from (1) to a finite element formulation. For example, the analysis may be carried out directly in terms of finite elements laid out in the reference configuration or. when the terms of (1) are transformed to integrals over V and S, to elements laid out in the cur- rent configuration. Particularly, an updated Lagrangian formulation is useful in which the varia- tional principle is transformed to the current configuration while the finite elements are fixed relative to material points and convect with the deformation. Additionally, there are various mea- sures of stress and strain which may be found convenient in particular constitutive representa- tions. Thus, while f can always be written as a linear expression in &-i/&Y and the rate of the

adopted stress measure (see Prager [ 12, 13 I and Hill [ 141 for discussions of relations among stress rates), it is often convenient to let the stress and deformation rate measures of the adopted con- stitutive relation enter directly into (1).

In view of these remarks, two types of transformations of (1) are of special interest for elastic- plastic analysis. First, in terms of the current configuration, true (or Cauchy) stress u, and rate of deformation D = 4 (&$/ax) + +(&/ax), there results [ 10, 111

s {(a* + e trD) : 6D - +U : 6[20 .D - (ai/ax) f (ax/ax)] } dV V

(7)

J.R. Rice et aLlRecent finite element studies in plasticity and fracture mechanics 413

for arbitrary 6i and associated 6D. Here again 6 and _? are nominal rates, but based on a reference configuration with which the current configuration is supposed to be coincident instantaneously. It is noted that t = e and

i=i+otrD-(C)i/&)-o (3)

when the reference and current configurations coincide; tr D denotes the trace (or first invari- ant) of D; u* is the co-rotational (or Jaumann) stress rate (e.g., [ 131)

a*=i-n.u+a-n (4)

where fi = $(&z/h) - + (a?/&) is the spin rate; the combination (a* + u tr 0) is the co-rotational rate, r*, of Kirchhoff stress where z = u dV/dV and the reference and current states coincide.

Another approach, which we will not develop in detail here, is to introduce work-conjugate symmetric stress and strain tensors S and E, defined [ 141 so that

(5)

for arbitrary &/ax, where E is any isotropic tensor function of (&/ax) * (&v/ax) - i.e., E is a material strain tensor. McMeeking and Rice [ 101 demonstrate the manner in which contribu-

tions to the tangential constitutive stiffness and initial stress stiffness vary in a compensatory

manner for different choices of strain measure. But for computation of E without resort to deter- mination of principal stretches, the most convenient and widely used form for E is the Green strain,

E = f [(ax/ax)' . (ax/ax> - II , (6)

and the conjugate stress measure is the second Piola-Kirchhoff stress

S = t. (ax/ax)- = det(aw/aX)(ax/aX)-l . u a (b/ax)- t. (7)

In terms of this (1) becomes [ 111

S{S:~~+fS:6[(~/ax)'.(a;/ax)]} dp = 1 d&dl/ +/f+dSO. vo vo so

(8)

There is a close connection between this principle, in terms of S and i, and the preceding ver- sion, eq. (2), in terms of r and D. It becomes apparent when the dyads T and D are referred to base vectors which are convected with the deformation but coincide, in the reference configura- tion, to the set of fixed base vectors to which S and E are supposed to be referred. Then in curvilinear tensor notation,

ii = pi, D, = iii. (9)

414 J.R. Rice et al./Recent finite element studies in plasticity and fracture tmchanics

Indeed, it is this observation which serves to show that the variational formulation in terms of S

and E, employed by Needleman [7, 81 and Hutchinson [ 151 coincides with that of (7). Further. although it was apparently not recognized at the time, a generalization of stress-strain relations for isotropic hardening due to Budiansky, used in [7, 8, 151 and phrased in terms of,?j and I?!,. is seen by virtue of the above remark to coincide with the classical Prandtl-Reuss equations when u* and D are used as the stress and strain rate.

In fact, all of our numerical examples are given in terms of the classical Prandtl-Reuss equa- tions and these have the form (when, e.g., a classical formulation like that of Hill I 161 is gener-

alized to the co-rotational stress rate)

D= 1 +v - e* E

ilO)

Here the last term is present only during plastic response; E is Youngs modulus; v is Poissons ratio; (I is the deviatoric stress; 0 is the equivalent strength in tension and is given such that

(2/3)G2 is the maximum value of u : e attained up to the present instant; I? is the slope of the true stress versus logarithmic plastic strain curve in a tensile test. This form of the Prandtl-Reuss

equations is invariant to superposed spins and properly embodies the approximately symmetric relation between true stress and logarithmic strain in tension and compression, as suggested by

experiments on annealed metals [ 161. More complicated expressions ar

*View more*